Chemical pulping of waste pineapple leaves fiber for kraft ... Pineapple leaves Pineapple...
Embed Size (px)
Transcript of Chemical pulping of waste pineapple leaves fiber for kraft ... Pineapple leaves Pineapple...
j m a t e r r e s t e c h n o l . 2 0 1 5;4(3):254–261
Available online at www.sciencedirect.com
Chemical pulping of waste pineapple leaves fiber for kraft paper production
Waham Ashaier Laftaha,∗, Wan Aizan Wan Abdul Rahamanb
a Department of Polymer Engineering, Faculty of Chemical Engineering, Universiti Teknologi Malaysia, Johor, Malaysia b Center for Composites, Universiti Teknologi Malaysia, Johor, Malaysia
a r t i c l e i n f o
Received 29 August 2014
Accepted 15 December 2014
Available online 15 January 2015
a b s t r a c t
The main objective of this study is to evaluate the implementation of acetone as a pulping
agent for pineapple leaves. Mixtures of water and acetone with concentration of 1%, 3%,
5%, 7%, and 10% were used. The effects of soaking and delignification time on the paper
properties were investigated. Thermal and physical properties of paper sheet were studied
using thermogravimetric analysis (TGA) and tearing resistance test respectively. The mor-
phological properties were observed using microscope at 200× magnification. The paper sheet produced from pulping with 3% acetone concentration shows the highest mechan-
ical properties. Papers strength was improved by increasing the delignification time. The
delignification time was reduced by cooking the pineapple leaves at a temperature of 118 ◦C
under applied pressure of 80 kPa which has remarkable effect on paper strength.
© 2014 Brazilian Metallurgical, Materials and Mining Association. Published by Elsevier
Editora Ltda. All rights reserved.
insufficient to sustain papermaking, and an alternative source
Pulp and paper industries have been considered the main con- sumers of natural resources (wood) and energy (electricity), including water, and significant contributors of pollutant dis- charges to the environment. The demand for paper and the unacceptable large ecological footprint of current paper pro- duction requires the need for alternatives. It was reported in 2004 that the annual paper consumption is 52.45 kg per per- son and was 16.32% greater than in 1991. The use of printing
and writing paper grew by more than 10% from 1980 to 2000 . In many parts of the world, local supplies of wood can- not support the demand for pulp. As a result, the search for
∗ Corresponding author. E-mail: firstname.lastname@example.org (W.A. Laftah).
http://dx.doi.org/10.1016/j.jmrt.2014.12.006 2238-7854/© 2014 Brazilian Metallurgical, Materials and Mining Associa
non-wood raw materials in papermaking industry has been given more attention due to the rising consumption of wood resource for the paper production. From 1970 to present time, the non-wood plant fiber pulping capacity has increased on a global basis two to three times as fast as the wood pulping capacity. It was also forecasted that during the next decade, the non-wood pulp production will annually grow at an aver- age of 6%, which is three times as fast as the production of pulp on wood basis . Initially, non-wood fiber pulping occurred in regions where wood supply had been reduced to levels
of fiber feedstock was mandatory. Non-wood fiber resources have the potential to complement conventional wood sup- plies. This is because, they are abundant, have short cycles
tion. Published by Elsevier Editora Ltda. All rights reserved.
dx.doi.org/10.1016/j.jmrt.2014.12.006 http://www.jmrt.com.br http://www.sciencedirect.com/science/journal/00000000 http://crossmark.crossref.org/dialog/?doi=10.1016/j.jmrt.2014.12.006&domain=pdf mailto:email@example.com dx.doi.org/10.1016/j.jmrt.2014.12.006
o l . 2
a T m n w [ j s i c n b a p r p p s p p m i u c w i c T a e a i r i t p t s [ k t t r a k p t t s t t
j m a t e r r e s t e c h n
nd rapid regeneration, and are of comparatively low price. herefore, non-wood fiber will play important roles in paper- aking as substitutes or complements to wood. Examples of
on-wood fiber resources available for paper production are heat-straw [3–5], rice-straw [6,7], sugarcane straw , reeds
9], bamboo , bagasse [11,12], kenaf , palm oil , and ute . Non-wood material, particularly wheat straw, was uccessfully exploited as the main raw material for papermak- ng in China because of the limited wood resource with forest overage of only 13.94% . By a wide margin, the leading on-wood plant fiber presently in use is straw, followed by agasse and bamboo. However, pineapple leaf fiber (PALF) is nother alternative non-wood fiber that can be used for paper roduction. There have been numerous studies carried out by esearchers on various aspects of PALF. PALF obtained from lants bearing edible fruits were examined for textile pur- oses, and blends of PALF with silk and polyester fibers were tudied . PALF have also been incorporated into thermo- lastic materials such as polypropylene and polyethylene to roduce biocomposite materials. The use of non-wood raw aterials provides several interesting advantages; specifically,
t allows wood raw materials to be saved for other more decent ses and hence deforestation and replanting to be alleviated. It an also reduce wood and cellulose fiber imports in countries ith a shortage of wood raw materials. Besides, users are
ncreasingly demanding papers that are obtained by using lean technologies or made from recycled or non-wood fiber. he current challenges of the pulp and paper industry are the chievement of affordable quality pulp while preserving the nvironment by using increasingly smaller amounts of water nd energy and gradually fewer raw materials . It is also mportant to minimize pollution from residual effluents that esults from cooking and bleaching of the raw materials. The ncreasing concern with the environment and its preserva- ion have exposed the need to replace the classical pulping rocess such as kraft and sulfite pulping which use sulfur con- aining reagents. This is due to the fact that the release of ulfur to the environment can cause serious pollution problem 6]. The new pulping processes using less polluting chemicals nown as the “organosolv” processes have been developed by he researchers to resolve the problem. During the last years, his large progress of process technology has been reported to educe the sulfur emissions by the pulp mills. Even though the bility to obtain pulp by using the organic solvents has been nown for some time, pilot plants and small-scale industrial lants exploiting them have only recently come into opera- ion. This has been the result of the shortage of alternatives o traditional procedures, which leads to the expenditure of ubstantial efforts in new processes. In fact, some processes hat use organic solvents are being reconsidered in response o the new economic and environmental order.
.1. Raw material
ineapple leaves were obtained from the plantation of alaysian Pineapple Industry Board (MPIB), Johor, Malaysia.
0 1 5;4(3):254–261 255
Industrial grade acetone with 65% purity was purchased from Krass Instrument and Services.
2.2. Sample preparation
Dried pineapple leaves were immersed in mixtures of ace- tone/water of 1%, 3%, 5%, 7%, and 10% (v/v) for 3 days to study the effect of acetone concentration on paper quality and to optimize the best mixture content for farther prepara- tion. The effect of soaking time was studied at interval times of 3, 7, 21 and 28 days. Mixture of 3% acetone was used to investigate the effect of cooking time on paper properties at 118 ◦C under applied pressure of 80 kPa. The pineapple leaf pulp was washed with water and disintegrated in a laboratory blender. The pulp was molded using mold and deckle. The paper was dried in the oven at 60 ◦C until the pulp was fully dried. Finally, the paper was pressed using the compression molding machine at 100 ◦C and pressure of 10 MPa to get even thickness of paper sheet.
The turbidity of spent liquor from puling process was determined using HACH Ratio/XR Turbidimeter. Thermogravi- metric analysis (TGA) was performed by using Mettler Toledo TGA/STDA851 at heating rate 10 ◦C/min with the temperature range between 30 ◦C and 800 ◦C. TGA was used to determine the thermal stability of cellulose and lignin in pineapple leaves and the paper sheet. The tearing resistance test or Elmendorf tear test was used to measure the internal tearing resistance of the paper rather than the edge-tear strength of paper. The test was carried out according to ASTM D1922 using the HT-8181 Elmendorf Tearing Strength Tester. The tearing resistance (expressed in grams-force, gf) of the paper was determined from the average tearing force and the number of sheets com- prising the test piece using following equation:
Tearing resistance, gf
= 16 ∗ 9.81 ∗ average scale reading ∗ gf capacity n ∗ 1600 gf
where gf capacity = 3200 g and number of plies, n = 1. Inverted Microscope LEICA DMIRM equipped with a digital
camera was used to study the morphology of the paper at 200× magnification. Morphological study was used to observe the fibers structure and their coarseness in the paper.
3. Results and discussion
Pulp quality is identified by the good strength, bleach abil- ity, high cellulose and